This preview shows pages 1–3. Sign up to view the full content.
This preview has intentionally blurred sections. Sign up to view the full version.
View Full Document
Unformatted text preview: ME 382 Lecture 23 13/iii/06 1 S TATISTICS OF F RACTURE • Very brittle materials have very small critical flaw sizes E.g., Consider a ceramic with K Ic ≈ 1 MPa √ m ( σ Y ≈ 14 GPa) Crack length for a “useful” strength of 150 MPa? Assume loading parameter for fracture: K I ! " # a ∴ Critical crack size for fracture when σ f = 150 MPa a cr ! K Ic 2 "# f 2 = 10 12 " $ 2.25 $ 10 16 ! 14 μ m ∴ Critical crack length ≈ grain size & random natural defects • Difficult to measure size of strengthlimiting flaw (problem is both small size, and the fact that there are lots of flaws of similar sizes) ∴ Use statistical methods to determine probability of failure Weakestlink statistics • Consider a chain made up of many brittle links Probability of failure of each link: P f = 0.3 / link Probability of survival of each link: P s = 1  P f = 0.7 ∴ For 1 link: P f = 0.3, P s = 0.7 For 2 links: P s = 0.7 x 0.7 = 0.49 ( P f = 0.51) For n links: P s = 0.7 n ⇒ P f = 1  (0.7) n ∴ P f ↑ as n ↑ • A general feature of nonredundant systems: P f ↑ as size ↑ • Brittle materials are full of flaws ME 382 Lecture 23 13/iii/06 2 • If one flaw is critical entire material fails: ∴ Weakestlink statistics apply • If volume flaws responsible for fracture: P f ↑ as volume ↑ • If surface flaws responsible for fracture: P f ↑ as surface area ↑ • Strength of glass limited by surface flaws Fresh glass fibers are very strong because they are very small ( ≈ 1 GPa)...
View
Full
Document
This note was uploaded on 03/20/2011 for the course ME 382 taught by Professor Garikipati during the Winter '08 term at University of Michigan.
 Winter '08
 garikipati

Click to edit the document details